Porosity Properties of the Conformers of Sodalite-like Zeolitic Imidazolate Frameworks.
Choi, Yejin; Noh, Kyungkyou; Lee, Jisu; Kim, Jaheon; Journal of the American Chemical Society 140 (2018) 14586–14589; doi:10.1021/jacs.8b08997

data_4133209
_publ_section_title
;
 Porosity Properties of the Conformers of Sodalite-like Zeolitic
 Imidazolate Frameworks.
;
_journal_issue                   44
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              14586
_journal_page_last               14589
_journal_paper_doi               10.1021/jacs.8b08997
_journal_volume                  140
_journal_year                    2018
_chemical_formula_moiety         'C6 H4 N6 O4 Zn [+ solvent]'
_chemical_formula_sum            'C6 H4 N6 O4 Zn'
_chemical_formula_weight         289.52
_chemical_name_common            a-ZIF-65(Zn)
_space_group_crystal_system      cubic
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            12
_cell_length_a                   17.3893(3)
_cell_length_b                   17.3893(3)
_cell_length_c                   17.3893(3)
_cell_measurement_reflns_used    9006
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      34.955
_cell_measurement_theta_min      1.656
_cell_volume                     5258.31(16)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELX-TL XP'
_computing_publication_material  'SHELX ciftab'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    SHELX-S
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker SMART CCD'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0417
_diffrn_reflns_av_unetI/netI     0.0583
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            9006
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         34.955
_diffrn_reflns_theta_min         1.656
_exptl_absorpt_coefficient_mu    1.410
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            'brick red'
_exptl_crystal_density_diffrn    1.097
_exptl_crystal_density_meas      ?
_exptl_crystal_description       block
_exptl_crystal_F_000             1728
_exptl_crystal_size_max          0.400
_exptl_crystal_size_mid          0.400
_exptl_crystal_size_min          0.250
_refine_diff_density_max         0.482
_refine_diff_density_min         -0.140
_refine_diff_density_rms         0.041
_refine_ls_abs_structure_details
;
 Flack x determined using 468 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.009(11)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.899
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     42
_refine_ls_number_reflns         2143
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.899
_refine_ls_R_factor_all          0.0697
_refine_ls_R_factor_gt           0.0320
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0308P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0665
_refine_ls_wR_factor_ref         0.0760
_reflns_Friedel_coverage         0.851
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     0.993
_reflns_number_gt                1326
_reflns_number_total             2143
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja8b08997_si_004.cif
_cod_data_source_block           a-ZIF-65(Zn)_RT
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_crystal_density_meas' value 'none' was changed to
'?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        5258.3(3)
_cod_database_code               4133209
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_min   0.602
_shelx_estimated_absorpt_t_max   0.719
_shelx_res_checksum              72244
_shelx_hkl_checksum              98522
_shelx_fab_checksum              19134